- Nano Idea
- Open Access
- Published:

# The effects of the size of nanocrystalline materials on their thermodynamic and mechanical properties

*Nanoscale Research Letters*
**volume 9**, Article number: 516 (2014)

## Abstract

This work has considered the intrinsic influence of bond energy on the macroscopic, thermodynamic, and mechanical properties of crystalline materials. A general criterion is proposed to evaluate the properties of nanocrystalline materials. The interrelation between the thermodynamic and mechanical properties of nanomaterials is presented and the relationship between the variation of these properties and the size of the nanomaterials is explained. The results of our work agree well with thermodynamics, molecular dynamics simulations, and experimental results. This method is of significance in investigating the size effects of nanomaterials and provides a new approach for studying their thermodynamic and mechanical properties.

## Background

Nanocrystalline materials exhibit novel physical and chemical properties which are different from the bulk behavior [1–5]. There are a great many theoretical and experimental investigations showing the size-dependent properties of nanomaterials. The typical trend is that the values of the thermodynamic and mechanical parameters fall with decreasing size of nanoparticles and nanostructure. These parameters include melting entropy and melting point [6–15], Debye temperature [10, 16, 17], cohesive energy [6, 18–23], diffusion activation energy [24, 25], amplitude of the thermal vibration [26, 27], thermal expansion coefficient [28–30], specific heat [31, 32], Young’s modulus [33–36], and mass density [37, 38]. All these behaviors are generally explained as a result of the high surface-to-volume ratio of nanomaterials. The proportion of atoms at the surface is no longer negligible and they possess higher energies than atoms in the interior of the particle. Over many decades, a huge volume of data has been established by experiments. However, the mechanism of the size effect is not clear because of the variation of these experimental results. Some excellent models have been developed using classical thermodynamics and modern molecular dynamics. However, most of them focus on only one or two parameters and give different explanations. As a result, there is no common understanding of the mechanism of size effects on nanomaterials. In particular, the question of whether it is possible to correlate the variation of the properties of nanomaterials has rarely received attention.

It is well known that the macroscopic thermodynamic and mechanical properties of crystalline materials are intrinsically determined by the binding energy. Therefore, the change of binding energy is the key to explaining the variation of the thermodynamic and mechanical properties of nanomaterials. In this paper, we present a model based on bond energy. By investigating the energy variation of a nanoparticle, an intrinsic interrelation between the thermodynamic and mechanical properties is achieved, revealing the effects of the size of nanocrystalline materials.

## Theoretical model

Figure 1 is a physical model used for the description of the energy change of a nanoparticle. In a perfect crystal (Figure 1A), there are no defects and all the atoms are located at their equilibrium lattice positions. The atomic radius is *r*_{
0
} and the density of the crystal is *ρ*_{
0
}. A nanoscale spherical particle, with radius *R*_{
0
} is taken out of the perfect crystal, as shown in Figure 1B. As bond cleavage of surface atoms takes place, the atoms on the outside of the particle depart from their equilibrium positions, resulting in compression of the particle. The radius of the outside particle decreases to *R.* The average gyration radius is *r* and the average density is *ρ*_{
R
}. Since mass is conserved in the above process, the mass of the sphere in the perfect crystal is equal to the mass of the outside particle. Therefore we have

and

where *N* is the overall number of atoms in the sphere. *η* is the atomic packing factor and can be determined by calculating the volume of the overall atoms in a unit cell *V*_{atoms}, and dividing this by the volume of the unit cell *V*_{cell} as follows, \eta =\frac{{V}_{\mathrm{atoms}}}{{V}_{\mathrm{cell}}}. The values of *η* are listed in Table 1.

In the above process, the energy of the outside particle would increase by an amount Δ*W*, including the surface energy *W*_{1} induced by the bond cleavage of the surface atoms and the lattice distortion energy *W*_{2} induced by the compression, due to the surface tension of the outside particle. This is summarized by

According to thermodynamics, the surface energy of the outside particle is equivalent to the increase of the Gibbs free energy. Therefore, the surface energy *W*_{1} can be calculated from *σ* ⋅ *ΔS.* Δ*S* is the surface area of the outside particle and *σ* is the surface tension. That is

In addition, the lattice distortion energy *W*_{2} can be calculated by considering the area change of one atom, namely *Nσ*(4*πr*_{0}^{2} - 4*πr*^{2}), where *N* is the overall number of atoms in the particle. This can be expressed by

Combining Equations 4 and 5, Equation 3 becomes

where *W*_{0} is defined as *W*_{0} = *N* ⋅ *σ* ⋅ 4 ⋅ *π* ⋅ *r*_{0}^{2}, referring to the overall bond energy or the standard cohesive energy of the spherical particle in the perfect crystal.

We define the term Δ*W/W*_{0} in Equation 6 as the energy variation rate of a nanoscale system. Thus, Equation 6 represents a size-dependent expression of the energy of the nanoparticle. Because Δ*W/W*_{0} is based on the bond energy, which intrinsically influences the macroscopic thermodynamic and mechanical properties of crystal materials, it is reasonable that Δ*W/W*_{0} is used as a general criterion to evaluate the properties of nanomaterials and to predict all those parameters related to bond energy.From Equation 6, it is clear that the energy is in inverse proportion to the radius of the spherical particle. Figure 2 plots the energy of Au, Co, W, and Ni as a function of the radius of the spherical particles. In each case, the rate of change of the energy gradually increases as the radius decreases, for radii greater than 15 nm. When the radius is around 5 to 15 nm, the rate of change of energy apparently increases with the decrease of the radius, being around 2.2% for Co, 2.43% for Ni, 2.03% for Au, and 2.39% for W, respectively, for radii around 15 nm. Sharp increases occur for radii less than 5 nm. The rates of change of energy for Co, Ni, Au, and W are 10.5%, 9.56%, 9.18%, and 10.9%, respectively, for radii around 2 nm.

Based on the principle of conservation of energy, the change of energy of the spherical particle is equal to the increase of the Gibbs free energy and the decrease of the cohesive energy when the spherical particle is removed from the perfect crystal. Therefore Equation 6 can be written as

where Δ*E* and *E*_{0} are the variational and standard cohesive energy of the nanomaterial, respectively. Δ*G* and *G*_{0} are the variational and standard Gibbs free energy, respectively, for a given value of Δ.

By using thermodynamic investigations, molecular dynamics simulations, and experimental methods, considerable research has been carried out in order to investigate the thermodynamic and mechanical properties of nanomaterials. There is much evidence to suggest that some parameters, such as melting point *T*_{
m
}, diffusion activation energy *Q*_{
d
}, heat of sublimation *L*_{
s
}, square Debye temperature *Θ*_{
D
}, and Young’s modulus *Y*, can be regarded as being directly proportional to the cohesive energy [1, 6, 8–30]. Heat capacity 1/*C*_{
m
} is proportional to square Debye temperature *Θ*_{
D
}[10]. It is well known that all these properties of crystalline materials are related to the bond energy. Therefore, a general expression can be used to describe the interrelation of the thermodynamic and mechanical parameters of nanomaterials, as follows:

Combining Equations 7 and 8, this general expression can be simplified to give

where, Δ*X* and *X*_{0} are the variational and standard thermodynamic and mechanical parameters, as determined by the bond energy, respectively.

## Discussion

In Figure 3A, our model (Equation 9) is compared to the result of a molecular dynamics simulation and other models, illustrated using the melting points of copper (Cu) nanoparticles. The best agreement is obtained between our model and the results of molecular dynamics simulation, as the particle radius is increased from 1.08 to 9.10 nm. Other models apparently underestimate the melting points of the copper nanoparticles. The ratio of *T*(*R*)*/T*_{
m
} in our model is slightly higher than the molecular dynamics simulation results, where the size-dependent melting points are lower than those of the experimental data [7]. Figure 3B shows a comparison of the Young’s modulus of copper nanoparticles obtained using Equation 9, with experimental results. Our model predicts the experimental data quite well.

Equations 8 and 9 reveal the essential relationships between the thermodynamic and mechanical properties of nanomaterials. With Equation 8, we can calculate the thermodynamic and mechanical parameters of nanomaterials using data obtained from either experiments or thermodynamic models. The size dependence of the heat capacity *C*_{
m
} and Young’s modulus *Y* for Ag, the Debye temperature *Θ*_{
D
} and diffusion activation energy *Q*_{
d
} for Au, calculated from Equation 8 using experimental melting point data *T*_{
m
}*,* are plotted in Figure 4. The prediction of our model (Equation 9) and the experimental results are also plotted for comparison. Good agreement is obtained between them.

## Conclusions

In summary, we have demonstrated the intrinsic interrelations between the thermodynamic and mechanical properties of nanomaterials using our bond energy model and previous results to characterize aspects of the size effects on nanocrystalline materials. Equation 9 not only presents a new model to better describe the thermodynamic and mechanical properties of nanomaterials, but also provides a new approach to obtain these parameters from others without requiring the formulation and proof of new models. In other words, most of the thermodynamic and mechanical properties of nanomaterials can be predicted by using either experimental data or results of a theoretical analysis. In this way, all factors, such as shape, crystal structure, defects and fabrication processes of nanomaterials, which must be considered when predicting the physical parameters of nanomaterials, can be obtained from experimental data. This is a significant advancement in the investigation and application of nanomaterials.

## References

Gleite H: Nanocrystalline materials.

*Prog Mater Sci*1989, 33: 223–315. 10.1016/0079-6425(89)90001-7Edelstein AS, Murday JS, Rath BB: Challenges in nanomaterials design.

*Prog Mater Sci*1997, 42: 5–21. 10.1016/S0079-6425(97)00005-4Giebultowicz T: Nanothermodynamics: breathing life into an old model.

*Nature*2000, 408: 299–301. 10.1038/35042654Tong WP, Tao NR, Wang ZB, Lu J, Lu K: Nitriding iron at lower temperatures.

*Science*2003, 299: 686–688. 10.1126/science.1080216Meyers MA, Mishra A, Benson DJ: Mechanical properties of nanocrystalline materials.

*Prog Mater Sci*2006, 51: 427–556. 10.1016/j.pmatsci.2005.08.003Sun CQ, Wang Y, Tay BK, Li S, Huang H, Zhang YB: Correlation between the melting point of a nanosolid and the cohesive energy of a surface atom.

*J Phys Chem B*2002, 106: 10701–10705. 10.1021/jp025868lDelogu F: Structural and energetic properties of unsupported Cu nanoparticles from room temperature to the melting point: molecular dynamics simulations.

*Phys Rev B*2005, 72: 205418.Zhang Z, Li JC, Jiang Q: Size effect on the freezing temperature of lead particles.

*J Mater Sci Lett*2000, 19: 1893–1895. 10.1023/A:1006778426038Guisbiers G, Buchaillot L: Modeling the melting enthalpy of nanomaterials.

*J Phys Chem C*2009, 113: 3566–3568.Zhu YF, Lian JS, Jiang Q: Modeling of the melting point, Debye temperature, thermal expansion coefficient, and the specific heat of nanostructured materials.

*J Phys Chem C*2009, 113: 16896–16900. 10.1021/jp902097fLi YJ, Qi WH, Huang BY, Wang MP, Xiong SY: Modeling the thermodynamic properties of bimetallic nanosolids.

*J Phys Chem Solids*2010, 71: 810–817. 10.1016/j.jpcs.2010.02.003Guisbiers G, Buchaillot L: Universal size/shape-dependent law for characteristic temperatures.

*Phys Lett A*2009, 374: 305–308. 10.1016/j.physleta.2009.10.054Guisbiers G: Size-dependent materials properties towards a universal equation.

*Nanoscale Res Lett*2010, 5: 1132–1136. 10.1007/s11671-010-9614-1Guisbiers G: Review on the analytical models describing melting at the nanoscale.

*J Nanoscience Lett*2012, 2: 8. 10.4236/snl.2012.21002Ganguli D: Size effect in melting: a historical overview.

*T Indian Ceramsoc*2008, 67: 49–62.Sadaiyandi K: Size dependent Debye temperature and mean square displacements of nanocrystalline Au, Ag and Al.

*Mater Chem Phys*2009, 115: 703–706. 10.1016/j.matchemphys.2009.02.008Jasiukiewicza C, Karpusb V: Debye temperature of cubic crystals.

*Solid State Commun*2003, 128: 167–169. 10.1016/j.ssc.2003.08.008Qi WH, Wang MP, Xu GY: The particle size dependence of cohesive energy of metallic nanoparticles.

*Chem Phys Lett*2003, 372: 632–634. 10.1016/S0009-2614(03)00470-6Safaei A: Shape, structural, and energetic effects on the cohesive energy and melting point of nanocrystals.

*J Phys Chem C*2010, 114: 13482–13496. 10.1021/jp1037365Jiang Q, Li JC, Chi BQ: Size-dependent cohesive energy of nanocrystals.

*Chem Phys Lett*2002, 366: 551–554. 10.1016/S0009-2614(02)01641-XYang CC, Li S: Investigation of cohesive energy effects on size-dependent physical and chemical properties of nanocrystals.

*Phys Rev B*2007, 75: 165413.Liu W, Liu D, Zheng WT, Jiang Q: Size and structural dependence of cohesive energy in Cu.

*J Phys Chem C*2008, 112: 18840–18845. 10.1021/jp7114143Vanithakumari SC, Nanda KK: A universal relation for the cohesive energy of nanoparticles.

*Phys Lett A*2008, 372: 6930–6934. 10.1016/j.physleta.2008.09.050Luo WH, Deng L, Su KL, Li KM, Liao GH, Xiao SF: Gibbs free energy approach to calculate the thermodynamic properties of copper nanocrystals.

*Phys B*2011, 406: 859–863. 10.1016/j.physb.2010.12.014Yu XH, Zhan ZL, Rong J, Liu Z, Li L, Liu JX: Vacancy formation energy and size effects.

*Chem Phys Lett*2014, 600: 43–45.Hou M, Azzaoui ME, Pattyn H, Verheyden J, Koops G, Zhang G: Growth and lattice dynamics of Co nanoparticles embedded in Ag: a combined molecular-dynamics simulation and Mössbauer study.

*Phys Rev B*2000, 62: 5117–5128. 10.1103/PhysRevB.62.5117Jiang Q, Ao ZM, Zheng WT: Temperature and size effects on the amplitude of atomic vibration of Co nanocrystals embedded in Ag matrix.

*Chem Phys Lett*2007, 439: 102–104. 10.1016/j.cplett.2007.03.047Gleiter H: Nanostructured materials: basic concepts and microstructure.

*Acta Mater*2000, 48: 1–29. 10.1016/S1359-6454(99)00285-2Zhao YH, Lu K: Grain-size dependence of thermal properties of nanocrystalline elemental selenium studied by X-ray diffraction.

*Phys Rev B*1997, 56: 14330–14337. 10.1103/PhysRevB.56.14330Yang CC, Xiao MX, Li W, Jiang Q: Size effects on Debye temperature, Einstein temperature, and volume thermal expansion coefficient of nanocrystals.

*Solid State Commun*2006, 139: 148–152. 10.1016/j.ssc.2006.05.035Rupp J, Birringer R: Enhanced specific-heat-capacity (cp) measurements (150–300 K) of nanometer-sized crystalline materials.

*Phys Rev B*1987, 36: 7888–7890. 10.1103/PhysRevB.36.7888Hellstern E, Fecht HJ, Fu Z, Johnson WL: Structural and thermodynamic properties of heavily mechanically deformed Ru and AlRu.

*J Appl Phys*1989, 65: 305–310. 10.1063/1.342541Lucas M, Mai W, Yang R, Wang ZL, Riedo E: Aspect ratio dependence of the elastic properties of ZnO nanobelts.

*Nano Lett*2007, 7: 1314–1317. 10.1021/nl070310gKulkarni AJ, Zhou M, Ke FJ: Orientation and size dependence of the elastic properties of zinc oxide nanobelts.

*Nanotechnology*2005, 16: 2749–2756. 10.1088/0957-4484/16/12/001Zhang LX, Huang HC: Young’s moduli of ZnO nanoplates: ab initio determinations.

*Appl Phys Lett*2006, 89: 183111. 10.1063/1.2374856Miller RE, Shenoy VB: Size-dependent elastic properties of nanosized structural elements.

*Nanotechnology*2000, 11: 139–147. 10.1088/0957-4484/11/3/301Safaei A: Size-dependent mass density of nanocrystals.

*Nano*2012, 71: 250009.Nanda KK: Size-dependent density of nanoparticles and nanostructured materials.

*Phys Lett A*2012, 376: 3301–3302. 10.1016/j.physleta.2012.10.001Warlimont M:

*Springer Handbook of Condensed Matter and Materials Data*. New York: Spinger Berlin Heidelberg; 2005.Keene BJ: Review of data for the surface tension of pure metals.

*Int Mater Views*1993, 38: 157–192.Jing Q, Yang CC: Size effect on the phase stability of nanostructures.

*Curr Nanoscience*2008, 4: 179–200. 10.2174/157341308784340949Guisbiers G, Kazan M, Overschelde OV, Wautelet M, Pereira S: Mechanical and thermal properties of metallic and semiconductive nanostructures.

*J Phys Chem C*2008, 112: 4097–4103. 10.1021/jp077371nSun CQ, Tay BK, Zeng XT, Li S, Chen TP, Zhou J, Bai HL, Jiang EY: Bond-order–bond-length–bond-strength (bond-OLS) correlation mechanism for the shape-and-size dependence of a nanosolid.

*J Phys Cond Matter*2002, 14: 7781–7795. 10.1088/0953-8984/14/34/301Streitz FH, Cammarata RC, Sieradzki K: Surface-stress effects on elastic properties. I. Thin metal films.

*Phys Rev B*1994, 49: 10699–10706. 10.1103/PhysRevB.49.10699Wong EW, Sheehan PE, Lieber CM: Nanobeam mechanics: elasticity, strength, and toughness of nanorods and nanotubes.

*Science*1997, 277: 1971–1975. 10.1126/science.277.5334.1971Xiong SY, Qi WH, Cheng YJ, Huang BY, Wang MP, Li YJ: Universal relation for size dependent thermodynamic properties of metallic nanoparticles.

*Phys Chem Chem Phys*2011, 13: 10652–10660. 10.1039/c0cp90161jXiao SF, Hu WY, Yang JY: Melting temperature: from nanocrystalline to amorphous.

*J Chem Phys*2006, 125: 184504. 10.1063/1.2371112Luo WH, Hu WY, Xiao SF: Size Effect on the thermodynamic properties of silver nanoparticles.

*J Phys Chem C*2008, 112: 2359–2369. 10.1021/jp0770155Kästle G, Boyen HG, Schröder A, Plettl A, Ziemann P: Size effect of the resistivity of thin epitaxial gold films.

*Phys Rev B*2004, 70: 165414.Buffat P, Borel JP: Size effect on the melting temperature of gold particles.

*Phys Rev A*1976, 13: 2287–2298. 10.1103/PhysRevA.13.2287Dick K, Dhanasekaran T, Zhang ZY, Meisel D: Size-dependent melting of silica-encapsulated gold nanoparticles.

*J Am Chem Soc*2002, 124: 2312–2317. 10.1021/ja017281aSambles JR: An electron microscope study of evaporating gold particles: the Kelvin equation for liquid and the lowering of the melting point of solid gold particles.

*Proc R Soc London A*1971, 324: 339–351. 10.1098/rspa.1971.0143Shibata T, Bunker BA, Zhang ZY, Meisel D, Vardeman CF, Gezelter JD: Size-dependent spontaneous alloying of Au-Ag nanoparticles.

*J Am Chem Soc*2002, 124: 11989–11996. 10.1021/ja026764rEdalati K, Horita Z: Correlations between hardness and atomic bond parameters of pure metals and semi-metals after processing by high-pressure torsion.

*Scr Mater*2011, 64: 161–164. 10.1016/j.scriptamat.2010.09.034

## Acknowledgements

This work was financially supported by the Natural Science Foundation of China (no. 51165016).

## Author information

### Authors and Affiliations

### Corresponding author

## Additional information

### Competing interests

The authors declare that they have no competing interests.

### Authors’ contributions

XH proposed the theoretical conception and drafted the manuscript. ZL participated in the theoretical design and helped to draft the manuscript. Both authors read and approved the final manuscript.

## Authors’ original submitted files for images

Below are the links to the authors’ original submitted files for images.

## Rights and permissions

**Open Access** This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (https://creativecommons.org/licenses/by/4.0), which permits use, duplication, adaptation, distribution, and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

## About this article

### Cite this article

Yu, X., Zhan, Z. The effects of the size of nanocrystalline materials on their thermodynamic and mechanical properties.
*Nanoscale Res Lett* **9, **516 (2014). https://doi.org/10.1186/1556-276X-9-516

Received:

Accepted:

Published:

DOI: https://doi.org/10.1186/1556-276X-9-516

### Keywords

- Size effects
- Nanocrystalline materials
- Thermodynamic
- Mechanical
- Bond energy